### Delft University of Technology

### Photogeneration Quantum Yield and Character of Free Charges and Excitons in PbSe

### Nanorods

Kulkarni, Aditya; Evers, Wiel H.; Van Waas, Thomas P.; Siebbeles, Laurens D.A. DOI

10.1021/acs.jpcc.0c00541

Publication date 2020

Document Version Final published version Published in

Journal of Physical Chemistry C

Citation (APA)

Kulkarni, A., Evers, W. H., Van Waas, T. P., & Siebbeles, L. D. A. (2020). Photogeneration Quantum Yield and Character of Free Charges and Excitons in PbSe Nanorods. Journal of Physical Chemistry C, 124(13), 7550-7557. https://doi.org/10.1021/acs.jpcc.0c00541

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

### Aditya Kulkarni, Wiel H. Evers, Thomas P. van Waas, and Laurens D. A. Siebbeles

### *

Cite This:J. Phys. Chem. C 2020, 124, 7550−7557 Read Online

### ACCESS

Metrics & More Article Recommendations### *

sı Supporting InformationABSTRACT: Lead selenide (PbSe) nanorods are of interest for applications in infrared
LEDs, lasers, and photovoltaics due to the possibility of tuning their band gap from the
far- to the near-infrared by decreasing their radius. We study the photogeneration
quantum yield and properties of free charges and excitons in PbSe nanorods using a
combination of time-resolved transient optical absorption and terahertz spectroscopy.
Photoexcitation predominantly leads to the formation of excitons and to a smaller
extent to free mobile charges. Theoretical analysis of the exprimental data yields an
exciton polarizability of 10−35C m2_{V}−1_{. The sum of the mobilities of a free electron and}
a hole is found to be close to 100 cm2V−1s−1. The high quantum yield of excitons
makes PbSe nanorods of interest as a gain material in near-infrared LEDs or lasers. To
use PbSe nanorods in photovoltaics, heterojunctions must be realized so that excitons
can dissociate into free charges.

## ■

INTRODUCTIONNanorods of PbSe are of interest due to the possibility of tuning their band gap from the far- to the near-infrared by a decrease in their radius. A band gap of close to 1 eV can be realized, which is ideal for solar cells, near-infrared detectors, and lasers.1−3 Interestingly, it has been found that a single energetic photon can excite two or more electrons in PbSe nanorods via a process known as carrier multiplication (CM).1,4 The eﬀect of CM in solar cells based on PbSe nanorods was found to lead to an external quantum eﬃciency of close to 120%.2

For optoelectronic applications as mentioned, it is important to understand to what extent photon absorption leads to the formation of free electrons and holes or mutually bound electrons and holes in the form of neutral excitons. The quantum yield of excitons ﬁrst increases when the photo-excitation density increases since then it becomes more likely that electrons and holes recombine to form excitons, as described by the Saha model.5−7 At very high density where the distance between excitons becomes comparable to their diameter, their spatial overlap causes screening of the electron−hole (e−h) Coulomb attraction, which can lead to the dissociation of excitons into free charges forming an e−h plasma.6,8Understanding the nature of photoexcited species as a function of density is of interest from a fundamental perspective as well as for optoelectronic applications of PbSe nanorods.

Theoretical calculations on PbSe nanowires have yielded exciton binding energies that strongly increase as their radius decreases, with a value that is as high as 0.4 eV for a radius near 1 nm.9 Transient optical absorption (TA) and photo-luminescence measurements do not directly reveal to what

extent photoexcitation leads to the formation of neutral excitons and free charges.1,4,10 However, according to the theoretical analysis of TA decay kinetics, excitons are the dominant species in longer PbSe nanorods.10,11

The aim of the current work is to determine to what extent
the photoexcitation of PbSe nanorods leads to free charges or
excitons and to determine the charge carrier mobility and the
exciton polarizability. We combine time-resolved TA
spectros-copy with terahertz (THz) photoconductivity measurements
for diﬀerent photoexcitation densities in order to distinguish
free charges from excitons. From an analysis of the TA and
THz photoconductivity data, it is inferred that photoexcitation
predominantly leads to the formation of excitons with a
polarizability of 10−35 C m2 _{V}−1_{. The quantum yield of}
photogenerated free charges is less than 0.13. The sum of the
mobility of an electron and hole moving in phase with the THz
electricﬁeld is as high as 91 ± 13 cm2V−1s−1.

## ■

METHODSSynthesis and Characterization of Nanorods. PbSe nanorods were synthesized by exactly following a previously reported procedure.12 Transmission electron microscopy (TEM) images were acquired using a Philips CM30T microscope operating at 200 kV. The nanorods were dispersed Received: January 20, 2020

Revised: March 10, 2020

Published: March 16, 2020

Downloaded via TU DELFT on May 4, 2020 at 11:06:45 (UTC).

in tetrachloroethylene for all spectroscopic measurements. The steady-state optical absorption was measured using a PerkinElmer Lambda 1050 spectrophotometer.

In the pump−probe laser experiments described below, it was found that stirring the sample solution or the prolonged duration of the measurements had no eﬀect on the results. This implies that the pump pulses do not cause charging or degradation of the nanorods.

Transient Optical Absorption Spectroscopy. The PbSe nanorod dispersion was photoexcited with 800 nm optical pulses with a duration of 180 fs. The reduced absorption (bleach) near the band gap due to presence of free electrons, holes, and excitons was probed by broadband optical pulses generated in a sapphire crystal using the laser system described in ref 12. The bleach of the low-energy absorption peak (Figure S2) was obtained from the transmitted probe light in

the presence of the pump pulse (Ion) and the absence of the pump pulse (Ioff) using the relation

13
i
k
jjjjj*I* y_{{}zzzzz
*I*
OD log ( )
( )
on
off
*λ*
*λ*
Δ =
(1)
The decay kinetics of the bleach was obtained by integrating
the entire peak in the 1100−1600 nm interval at each pump−
probe delay time.

Optical Pump−THz Probe Spectroscopy. The PbSe nanorod dispersion was photoexcited with 800 nm optical pump pulses of 60 fs width. The photogenerated free electrons, holes, and excitons were probed by single-cycle THz pulses. Single-cycle THz pulses were generated in a nonlinear crystal ZnTe via optical rectiﬁcation of 60 fs pulses of wavelength 800 nm similar to that in previous work.14,15The THz pulse was detected in a ZnTe crystal by spatially overlapping it with a chirped optical laser pulse centered at 800 nm so that the Figure 1.Structural and optical characterization. (A) TEM image of PbSe nanorods. (The scale bar represents 60 nm.) (B) Optical absorption spectrum of the PbSe nanorod dispersion exhibiting a low-energy absorption peak at 1395 nm.

Figure 2.TA spectroscopy results. (A)ΔOD after photoexcitation at 800 nm. (B) The bleach rises more slowly at higher excitation density. (C) Initial bleach signal,A, obtained by averaging over a time range of 5−10 ps and the long-time bleach, B, obtained by averaging over 2.0−2.5 ns plotted versus the excitation density. (D) Values ofNi=A/B (red markers plotted on the left axis) and N0(black curve plotted on the right axis) as

a function of the number of incident photons per cm2_{,}_{j}

0, (bottom axis) and the excitation density (top axis).

The Journal of Physical Chemistry C pubs.acs.org/JPCC Article

https://dx.doi.org/10.1021/acs.jpcc.0c00541

J. Phys. Chem. C 2020, 124, 7550−7557 7551

refractive index of the solvent,c being the speed of light in a
vacuum, andε_{0}being the vacuum permittivity.

The real part of the THz conductivity signal,SR(t), is related to the quantum yield (i.e., the number of pairs of free electrons and holes per absorbed photon,ϕ(t), present at time t after the pump pulse) and the sum of the real component of the electron and hole mobilityμe + μh ≡ μR of charges moving along the direction of the nanorod according to7,14,16,18

*S t* *t* *RL*
*eN*
( ) ( )
R R
R
a
*ϕ* *μ* *σ*
= = Δ
(3)
In eq 3, e is the elementary charge and Na is the number of
absorbed photons per unit area in the nanorod dispersion,
which is referred to as the photoexcitation density. FactorR in

eq 3takes into account the eﬀects of the angle between the
polarization direction of the pump laser pulse and the direction
of the THz electricﬁeld with respect to the randomly oriented
axes of the nanorods. The transition dipole moment for an
optical transition is parallel or perpendicular to the axis of the
nanorod, so the optical absorption cross section of a nanorod
depends on the angleΘ of its axis with respect to the pump
polarization direction according to cos2_{(}_{Θ) or sin}2_{(}_{Θ),}
respectively. Assuming that the THz conductivity
perpendic-ular to the axis of a nanorod is negligible, the THz conductivity
of a nanorod at an angleΩ with the THz ﬁeld is proportional
to cos2_{(}_{Ω). Taking this into account, the factor R can be}
determined from the ratio of the THz conductivity measured
with the pump laser polarization parallel and perpendicular to
the THzﬁeld, respectively. From such measurements, it was
found thatR = 3.3 (SI section 1). The imaginary conductivity
signal SI(t) due to free electrons and holes, as well as the
polarizability of excitons along the direction of the nanorod, is
given by7,18
*S t* *t* *t*
*e* *R*
*L*
*eN*
( ) ( ) 1 ( )
I I
I
a
*ϕ* *μ* *ϕ* *αω* *σ*
= + [ − ] = Δ
(4)
with μI being the sum of the imaginary electron and hole
mobility,α being the polarizability of an exciton, and ω being
the radian frequency of the THzﬁeld.

## ■

RESULTS AND DISCUSSIONAccording to an analysis of the TEM image inFigure 1A, the nanorods have a diameter of 4.0± 0.8 nm and a length of 51 ± 11 nm. The optical absorption spectrum of the PbSe nanorod dispersion is shown inFigure 1B. The absorption peak at lower photon energy is maximized at 1395 nm.

Transient Optical Absorption Spectroscopy.Figure 2A shows the time-dependent bleach, ΔOD, after photoexciting the PbSe nanorod dispersion with 800 nm pump pulses with a duration of 180 fs (MethodsandFigure S2). As expected, the initial amplitude of the bleach increases with the excitation density (deﬁned as the number of absorbed pump photons per

during this time is due to energetic relaxation (cooling) of the initially hot electrons and holes to the band edge. At the lowest excitation density, this is observed to occur within 1 ps, similar to previous results.10With increasing density, cooling appears to be prolonged and takes about 4 ps at the highest density. This can be understood as follows.21Net cooling of the charge carrier population occurs by the emission of phonons. At a higher charge carrier density, a larger number of phonons is emitted, and the nuclear lattice heats up more than for a low charge carrier density. Consequently, at higher density the reabsorption of phonons by charge carriers is more likely and the cooling time becomes longer.

The initial average number of free e−h pairs and excitons can be determined from the ratio of the maximum bleach amplitude,A, at short time after photoexcitation and the bleach at long time,B, when Auger recombination is complete and a single e−h pair or exciton is left in a photoexcited nanorod.4,22,23 In Figure 2C, values of A are shown, as obtained by averaging the bleach over a time range of 5−10 ps, which is suﬃciently long after the pump pulse so that charges have cooled to the band edge. The values ofB inFigure 2C were obtained by averaging over 2.0−2.5 ns, during which the bleach in Figure 2A can be attributed to single e−h pairs or

excitons since the bleach exhibits no signiﬁcant decay. The values of A ﬁrst increase linearly with excitation density, reﬂecting that the number of e−h pairs and excitons is directly proportional to the excitation density. At higher excitation density, the increase becomes sublinear, which is attributed to decay by Auger recombination on a time scale shorter than 10 ps. The value ofB ﬁrst increases with excitation density due to the fact that more nanorods are photoexcited, while it eventually saturates when all nanorods are excited and thus contains one e−h pair or exciton at longer times.

Figure 2D shows ratio A/B as a function of the incident (bottom axis) and absorbed (top axis) number of photons per unit area. The ratioA/B is equal to the average initial number, Ni, of e−h pairs and excitons per photoexcited nanorod in the time range of 5−10 ps. The value of Niis equal to the average number of absorbed photons per photoexcited nanorod, N0, provided the density of e−h pairs and excitons in the nanorods is low enough that Auger recombination at times of less than 10 ps is insigniﬁcant. The number of absorbed photons per nanorod follows a Poisson distribution so that the average initial number of e−h pairs and excitons per nanorod is equal toj0σabs, withj0being the number of incident pump photons per unit area andσabs being the absorption cross section at a pump wavelength of 800 nm. The initial average number of e− h pairs and excitons per photoexcited nanorod is then equal to

*N* *j*
*e*
(1 *j* )
0 0 abs
0 abs
*σ*
=
− − *σ* (5)

Fitting eq 5to the ratio A/B for those densities at which A increases linearly with the excitation density (so that Auger recombination does not aﬀect A) yields the black curve in

Figure 2D with σabs = (5.0 ± 0.4) × 10−14 cm2. At higher excitation density,A/B is smaller than N0, which is attributed to the decay of e−h pairs and excitons by Auger recombination on a time scale shorter than 10 ps.

For the value of σabs at 800 nm obtained from theﬁt, the
optical absorption spectrum inFigure 1B yields an absorption
cross section at the maximum of the low-energy peak equal to
2× 10−14 cm2. Cunningham et al. reported a cross section of
7.2× 10−15cm2at the low-energy peak for PbSe nanorods with
volume 240 nm3_{.}19

Taking our value ofσ_{abs}at the low-energy
peak and assuming it to scale linearly with the nanorod
volume,24 which is 640 nm3 for our nanorods,4,19 yields an
absorption cross section of 7.5× 10−15 cm2for nanorods of
volume 240 nm3_{, which agrees with the value reported by}
Cunningham et al.19

THz Spectroscopy. THz photoconductivity experiments were conducted to determine to what extent photoexcitation leads to the formation of free e−h pairs and neutral excitons.

Figure 3 shows THz photoconductivity data obtained by photoexcitation of the PbSe nanorods with 800 nm pump pulses of 60 fs duration. The real component of the THz conductivity is due to the motion of charges with velocity in phase with the THzﬁeld, and the imaginary part of the THz conductivity is due to the out-of-phase velocity resulting from the backscattering of charges and the polarizability of excitons (Methods).16,17,25

Figure 3A shows the real (positive) and imaginary (negative) components of the diﬀerential THz signal averaged over frequencies (f = ω/2π) in the range of 0.5−1.2 THz as a function of time after the pump pulse. To realize the

absorption of at most one photon per nanorod, it was necessary to use low excitation densities, leading to a relatively large noise level in the THz signals. The diﬀerential THz signal is directly proportional to the conductivity or, equivalently, the density of e−h pairs and excitons weighted by their mobility and polarizability, respectively (Methods). The real compo-nent is attributed to the presence of free mobile charge carriers only. Excitons do not contribute to the real component since the calculated exciton binding energy in PbSe nanowires of diameter 4 nm is as high as 0.154 eV (ref9); consequently, excitation to a higher exciton level will largely exceed the THz photon energy (1 THz = 4 meV). At higher excitation density, the imaginary THz signal decays faster than the real component. This must be due to the fact that excitons also contribute to the imaginary component. Hence, from the data in Figure 3A, we can conclude that both e−h pairs and excitons are produced by photoexcitation.

Figure 3B shows the real component of the product of the quantum yield of e−h pairs, ϕ(t), and the sum of the mobility of an electron and a hole (i.e.,SR(t) = ϕ(t)μR). Note that the quantum yield is the number of e−h pairs per absorbed pump photon at timet after the pump pulse. It can be seen that SR decays faster at higher excitation density, which is due to the enhanced Auger recombination of charges. The reduction of the magnitude ofSRwith excitation density may result from a decrease in the quantum yield of charges and/or a reduction in the charge mobility at higher density. This reduction will be addressed further in the next section. The initial values of the quantum-yield-weighted real mobility,SR(t), averaged over t in the interval 5−10 ps are shown in Figure 3C as a function of the average initial number of e−h pairs and excitons per nanorod,Ni.

Figure 3.THz photoconductivity results. (A) Real (positive) and imaginary (negative) diﬀerential THz signals after photoexcitation at 800 nm for excitation densities as indicated. (B) Quantum-yield-weighted real mobility of free charges obtained from the data inFigure 3A. (C) Initial quantum-yield-weighted real mobility of charges,SR,i(red markers), and product of the quantum yield calculated from the Saha model and the

ﬁtted mobility of charges. (D) Quantum yields of charges and excitons versus Nicalculated from the Saha model.

The Journal of Physical Chemistry C pubs.acs.org/JPCC Article

https://dx.doi.org/10.1021/acs.jpcc.0c00541

J. Phys. Chem. C 2020, 124, 7550−7557 7553

Quantum Yield and Mobility of Charges and
Polar-izability of Excitons. According to the 1D Saha model, the
equilibrium between the density of pairs of free charges nq=
ϕiNi/L and excitons nX= (1− ϕi)Ni/L on a nanorod of length
L is described by26
i
k
jjjjj y_{{}zzzzz i_{k}jjjjj y_{{}zzzzz
*n*
*n* *K*
*m k T* *E*
*k T*
2
exp
*X*
*X*
q2 _{B}
2
1/2
B
*π*
= = *
ℏ
−
(6)
The quantum yield of e−h pairs ϕi is obtained from the real
THz conductivity data 5−10 ps after the pump pulse inFigure
3C. The reduced eﬀective mass of electrons and holes m =
0.112m0 is obtained from the calculated valence and
conduction band dispersion (SI Section 5) reported in the
literature,9 and the exciton binding energyEX = 0.154 eV is
also taken from the literature.9kBis the Boltzmann constant,ℏ
is the reduced Planck constant, andT is the temperature (293
K). Usingeq 6, the quantum yield of e−h pairs is found to be

### (

1 1### )

*i*

*KL*

*N*

*N*

*KL*2 4

*i*

*i*

*ϕ =* − − + . Fitting the product ϕiμR to the
data inFigure 3C withK calculated fromeq 6and the mobility
of an e−h pair as an adjustable parameter yields μR= 91± 13
cm2_{V}−1_{s}−1_{. The}_{ﬁt reproduces the experimental values of S}

R,i up toNi= 6. The reduction ofSR,iwithNican be attributed to a decrease in the quantum yield of e−h pairs (and thus higher quantum yield of excitons), as described by the Saha model (eq 6). Note thatﬁlling of traps with charges would lead to an increase in SR,i when Ni increases. Hence, trap ﬁlling is not important. For higher values ofNi, the experimental values of SR,i are lower than those from the ﬁt. This can be due to a decrease in the charge mobility since at higher density the mutual scattering of charges in a rod ofﬁnite length will reduce their mobility. Figure 3D shows the quantum yield of e−h pairs and that of excitons. It is seen that photoexcitation leads

mainly to the formation of excitons with a quantum yield exceeding 0.85 even at lowNi.

The real mobility of charges obtained above can be limited
by scattering at the ends of the nanorod. The alternating
current (AC) charge carrier mobilityμac(f) at THz frequency f
on a nanorod of ﬁnite length L can be related to the direct
current (DC) mobility μdc of a charge on an inﬁnitely long
nanowire according to27−29
*f* *C*
*C*
( ) 8
1
*p*
*p*
*k T*
*eL* *f* *p*
ac dc
0
2
i
2
2
B dc
2

### ∑

*μ*=

*μ*−

*μ*

*π*= ∞ − (7) withe being the elementary charge and

*Cp*2

### (

*p*

### )

1 2

*π*

= + .

Equation 7yields for the real and imaginary components

### ( )

*f*

*C*

*C*( ) 8 1

*p*

*p*

*k T*

*eL*

*f*

*p*ac R dc 0 2 2 2 4 B dc 2

### ∑

*μ*=

*μ*+

*μ*= ∞ − (8)

_{π}### ( )

*f*

*C*

*C*( ) 8 1

*p*

*p*

*k T*

*eL*

*f*

*k T*

*eL*

*f*

*p*ac I dc 0 2 2 2 2 4 B dc 2 B dc 2

### ∑

*μ*=

*μ*+

*μ*

*π*

*μ*

*π*= ∞ − (9)

Figure 4A shows the real and imaginary parts of the ac
mobility forf = 0.8 THz (the central frequency at which the
experimental data inFigures 3and4were obtained) calculated
from eqs 8 and 9 for a nanorod length of L = 51 nm as a
function ofμ_{dc}. The experimental AC mobility is reproduced
for 115 and 2265 cm2 V−1 s−1. The correct value can be
determined by also considering the initial imaginary THz
conductivity data in Figure 4B, which correspond to

*S*I,*i*=*ϕμi* I + [ −1 *ϕi*] *e*
*αω*

(eq 4), with μI being the sum of the imaginary electron and hole mobility, α being the Figure 4.Theoretical modeling. (A) Calculated real and imaginary components ofμacas a function ofμdcat frequency 0.8 THz for a nanorod of

length 51 nm. (B) ExperimentalSI,ivalues (markers), obtained by averaging over 5−10 ps after the laser pump pulse and ﬁt with μI= 25 cm2V−1

s−1andα as an adjustable parameter (drawn curve). (C) Experimental (markers) and theoretical (drawn black curves) decays of N as a function of time with the initial condition for a Poisson distribution of excitons; seeeq 10. (D) Decay withN = Nias the initial condition ineq 10forN ≥ 6.

polarizability of an exciton, andω being the radian frequency
of the THzﬁeld. Fitting SI,i with the quantum yield from the
Saha model andμI= 25 cm2V−1s−1(corresponding toμdc=
115 cm2_{V}−1_{s}−1_{) yields the drawn curve in}_{Figure 4}_{B with}_{α =}
(0.9 ± 0.1) × 10−35 C m2 V−1. The ﬁt reproduces the
experimental data with the exception of high densities. By
contrast, takingμdc= 2265 cm2V−1s−1and the corresponding
μI = 404 cm2 V−1 s−1 fails to reproduce the measured data
(Figure S6). Therefore, we conclude thatμ_{dc} = 115 cm2 _{V}−1
s−1. Since this value is close to the measured real THz mobility,
the eﬀect of scattering of charges at the ends of a nanorod is
very small when probed at a frequency near 0.8 THz. The
mobility from the present work is comparable to that reported
previously for as-grown colloidal PbSe nanowires in a
ﬁeld-eﬀect transistor device.30 Interestingly, the mobility in the
device could be enhanced by about an order of magnitude via
coating the nanowires with SiO2.30Unfortunately, after being
coated the nanowires are no longer solution processable. The
mobility of charges in the colloidal PbSe nanorods is more
than 1 order of magnitude higher than for amorphous silicon,
making the nanorods of interest for electronic applications.

In the analysis described above, it was assumed that either
the electron or the hole is mobile, which gives a lower limit to
the exciton polarizability. Since the eﬀective masses of
electrons and holes are almost equal (SI Section 5), it is
reasonable to assume that electrons and holes have the same
mobility of 45 cm2V−1s−1. In that case, we obtainμI= 12 cm2
V−1s−1and an upper limit to the exciton polarizability equal to
α = 1.1 × 10−35 _{C m}2 _{V}−1_{. The exciton polarizability can be}
estimated theoretically using *e a*

*E* *E*
theory
22B
2
1 0
*α* = _{−} ,31 where the

summation over all higher exciton states is reduced to the
ﬁrst only, the transion dipole moment is taken to be equal to
the calculated exciton Bohr radiusaB= 2.2 nm, andE1− E2is
taken to be equal to the exciton binding energy for PbSe
nanowires with 4 nm diameter, as mentioned above.9 This
givesα_{theory}= 10−35C m2_{V}−1_{, which is in close agreement with}
the experimental result of (1.0± 0.1) × 10−35C m2V−1. The
agreement between the experimental polarizability and that
theoretically estimated from the calculated Bohr radius and
exciton binding energy supports the validity of the theoretical
model for the electronic structure used in ref 9. The much
smaller Bohr radius than for bulk PbSe (46 nm)9is attributed
to geometrical conﬁnement in a nanowire and the lower
dielectric constant of the surrounding medium (i.e., the surface
ligands and the solvent).

As discussed above, photoexcitation of the PbSe nanorods leads mainly to excitons (Figure 3D). Hence, the optical bleach at the band gap (ΔOD inFigures 2A,S2, andS3) can lead to a good approximation taken as a measure of the average number of excitons per nanorod, which we denote asN. As discussed above, for low excitation densitiesNi=N0≤ 6, the maximum bleach at short time directly reﬂects the average number of photoexcitations per nanorod. For these densities, the transients in Figure 4C,D were obtained by scaling the measured bleach (ΔOD) such that they have magnitude j0σabs at the maximum. At higher densities, this procedure is not valid due to Auger recombination of hot charge carriers prior to having relaxed to the band gap. This causes the maximum bleach at short time to be smaller thanj0σabs, as seen inFigure

2D. Fortunately, at these higher densities all nanorods are photoexcited and the bleach can be scaled such that at long timesN = 1.

Taking into account the Auger recombination of excitons,
the time-dependent average number of excitons per nanorod is
given by32
Ä
Ç
ÅÅÅÅÅ
ÅÅÅ ikjjj
y
{
zzz É_{Ö}ÑÑÑÑÑ_{ÑÑÑ}
*N t*( ) *A* exp *i* 1 *i* *k* *t*
2( 1)
*i*
*i*
1
2
A

### ∑

= − − = ∞ (10) withk2Abeing the Auger recombination rate for two excitons in a nanorod. The coeﬃcients ineq 10are equal to32*A* *N e* *i* *N*
*j*
*i* *j*
*i* *j*
(2 1) ( )
(2 )
*i*
*i* *N*
*j*
*j*
0

### ∑

= − ! Γ + Γ + − = ∞ (11) By taking the initial value of the number of photogenerated excitons in a nanorod equal toN = joσabs, we could reproduce the measured optical bleach transients untilN = 6 with a value ofk2A= 3× 109s−1(Figure 4C). ForN > 6, the ﬁtted transients exceed the experimental results at shorter times. This is attributed to the Auger recombination of hot e−h pairs before they reach the band edge so that the maximum in the measured transient does not represent the initial number of photoexcitations. Hence, for the transients at higher density such thatN > 6, we take NifromFigure 2D as the initial value N ineq 11, yielding the curves shown inFigure 4D. Theﬁtted curves inFigure 4D obtained withk2A= 3× 109s−1agree with the experimental data. From this, we infer that the Auger recombination of hot e−h pairs reduces the initial average number of excitons at the band gap in a nanorod while approximately maintaining a Poisson distribution, which is the initial condition for eq 10. Results for other densities are shown inFigure S7. The biexciton lifetime of 1/k2A = 330 ps obtained as described above is somewhat longer than the value of 210 ps reported for shorter nanorods of average length 25 and 4 nm diameter.10This can be understood since in longer nanorods the spatial overlap between two excitons will be smaller than in shorter nanorods, which enhances the lifetime before Auger recombination.## ■

CONCLUSIONSPhotoexcitation of the PbSe nanorods studied predominantly
leads to excitons rather than free e−h pairs. The exciton
polarizability of 10−35C m2V−1inferred from the experiments
agrees with the polarizability from a theoretical estimate. The
sum of the mobility of an electron and hole moving in phase
with the THz electricﬁeld is as high as 91 ± 13 cm2_{V}−1_{s}−1_{.}
For higher photoexcitation density, the photoconductivity is
strongly aﬀected by mutual interactions between charges and
excitons, leading to a lower charge mobility. The high quantum
yield of excitons makes PbSe nanorods of interest as a gain
material in near-infrared LEDs or lasers. For the use of PbSe
nanorods in solar cells, heterojunctions must be realized so
that excitons can dissociate into free charges.

## ■

ASSOCIATED CONTENT### *

sı Supporting InformationThe Supporting Information is available free of charge at

https://pubs.acs.org/doi/10.1021/acs.jpcc.0c00541.

Determination of factorR in eqs 3and 4 of the main text, spectral bleach for diﬀerent values of Ni, TA spectroscopy data, THz photoconductivity data, deter-mination of the eﬀective masses of electrons and holes, ﬁt to the imaginary component of the THz signal, and simulated decay of optical bleach (PDF)

The Journal of Physical Chemistry C pubs.acs.org/JPCC Article

https://dx.doi.org/10.1021/acs.jpcc.0c00541

J. Phys. Chem. C 2020, 124, 7550−7557 7555

HZ Delft, The Netherlands

Wiel H. Evers − Optoelectronic Materials Section, Department of Chemical Engineering, Delft University of Technology 2629 HZ Delft, The Netherlands

Thomas P. van Waas − Optoelectronic Materials Section, Department of Chemical Engineering, Delft University of Technology 2629 HZ Delft, The Netherlands

Complete contact information is available at:

https://pubs.acs.org/10.1021/acs.jpcc.0c00541

Author Contributions

W.H.E. synthesized the samples. A.K. performed terahertz photoconductivity and transient optical absorption spectros-copy measurements. A.K. and L.D.A.S. analyzed the exper-imental results. T.P.v.W. provided theoretical support. L.D.A.S. supervised the work and wrote the manuscript with A.K. All authors discussed the results and commented on the manuscript.

Notes

The authors declare no competingﬁnancial interest.

## ■

ACKNOWLEDGMENTSThis work is part of the research programme of the Foundation for Fundamental Research on Matter (FOM), which is part of The Netherlands Organisation for Scientiﬁc Research (NWO) in the program “Designing Dirac Carriers in Semiconductor Honeycomb Superlattices”.

## ■

REFERENCES(1) Cunningham, P. D.; Boercker, J. E.; Foos, E. E.; Lumb, M. P.; Smith, A. R.; Tischler, J. G.; Melinger, J. S. Enhanced Multiple Exciton Generation in Quasi-One-Dimensional Semiconductors. Nano Lett. 2011, 11, 3476−3481.

(2) Davis, N. J. L. K.; Böhm, M. L.; Tabachnyk, M.; Wisnivesky-Rocca-Rivarola, F.; Jellicoe, T. C.; Ducati, C.; Ehrler, B.; Greenham, N. C. Multiple-Exciton Generation in Lead Selenide Nanorod Solar Cells with External Quantum Efficiencies Exceeding 120%. Nat. Commun. 2015, 6, 8259.

(3) Talebi, H.; Dolatyari, M.; Rostami, G.; Manzuri, A.; Mahmudi, M.; Rostami, A. Fabrication of Fast Mid-Infrared Range Photo-detector Based on Hybrid Graphene−PbSe Nanorods. Appl. Opt. 2015,54, 6386−6390.

(4) Padilha, L. A.; Stewart, J. T.; Sandberg, R. L.; Bae, W. K.; Koh, W. K.; Pietryga, J. M.; Klimov, V. I. Carrier Multiplication in Semiconductor Nanocrystals: Influence of Size, Shape, and Composition.Acc. Chem. Res. 2013, 46, 1261−1269.

(5) Kaindl, R. A.; Hägele, D.; Carnahan, M. A.; Chemla, D. S. Transient Terahertz Spectroscopy of Excitons and Unbound Carriers in Quasi-Two-Dimensional Electron-Hole Gases. Phys. Rev. B: Condens. Matter Mater. Phys. 2009, 79, 045320.

(6) Hangleiter, A.; Jin, Z.; Gerhard, M.; Kalincev, D.; Langer, T.; Bremers, H.; Rossow, U.; Koch, M.; Bonn, M.; Turchinovich, D. Efficient Formation of Excitons in a Dense Electron-Hole Plasma at

Nanowires. Phys. Rev. B: Condens. Matter Mater. Phys. 2010, 82, 195313.

(10) Yang, J.; Hyun, B.-R.; Basile, A. J.; Wise, F. W. Exciton Relaxation in PbSe Nanorods.ACS Nano 2012, 6, 8120−8127.

(11) Aerts, M.; Spoor, F. C. M.; Grozema, F. C.; Houtepen, A. J.; Schins, J. M.; Siebbeles, L. D. A. Cooling and Auger Recombination of Charges in PbSe Nanorods: Crossover from Cubic to Bimolecular Decay.Nano Lett. 2013, 13, 4380−4386.

(12) Placencia, D.; Boercker, J. E.; Foos, E. E.; Tischler, J. G. Synthesis and Optical Properties of PbSe Nanorods with Controlled Diameter and Length.J. Phys. Chem. Lett. 2015, 6, 3360−3364.

(13) Spoor, F. C. M.; Kunneman, L. T.; Evers, W. H.; Renaud, N.; Grozema, F. C.; Houtepen, A. J.; Siebbeles, L. D. A. Hole Cooling Is Much Faster Than Electron Cooling in PbSe Quantum Dots.ACS Nano 2016, 10, 695−703.

(14) Evers, W. H.; et al. High Charge Mobility in Two-Dimensional Percolative Networks of PbSe Quantum Dots Connected by Atomic Bonds.Nat. Commun. 2015, 6, 8195.

(15) Kulkarni, A.; Evers, W. H.; Tomić, S.; Beard, M. C.; Vanmaekelbergh, D.; Siebbeles, L. D. A. Efficient Steplike Carrier Multiplication in Percolative Networks of Epitaxially Connected PbSe Nanocrystals.ACS Nano 2018, 12, 378−384.

(16) Ulbricht, R.; Hendry, E.; Shan, J.; Heinz, T. F.; Bonn, M. Carrier Dynamics in Semiconductors Studied with Time-Resolved Terahertz Spectroscopy.Rev. Mod. Phys. 2011, 83, 543−586.

(17) Joyce, H. J.; Boland, J. L.; Davies, C. L.; Baig, S. A.; Johnston, M. B. A Review of the Electrical Properties of Semiconductor Nanowires: Insights Gained from Terahertz Conductivity Spectros-copy.Semicond. Sci. Technol. 2016, 31, 103003.

(18) Tomar, R.; Kulkarni, A.; Chen, K.; Singh, S.; van Thourhout, D.; Hodgkiss, J. M.; Siebbeles, L. D. A.; Hens, Z.; Geiregat, P. Charge Carrier Cooling Bottleneck Opens up Nonexcitonic Gain Mecha-nisms in Colloidal Cdse Quantum Wells.J. Phys. Chem. C 2019, 123, 9640−9650.

(19) Cunningham, P. D.; Boercker, J. E.; Placencia, D.; Tischler, J. G. Anisotropic Absorption in PbSe Nanorods. ACS Nano 2014, 8, 581−590.

(20) Schaller, R. D.; Klimov, V. I. High Efficiency Carrier Multiplication in PbSe Nanocrystals: Implications for Solar Energy Conversion.Phys. Rev. Lett. 2004, 92, 186601.

(21) Shah, J. Ultrafast Luminescence Studies of Carrier Relaxation and Tunneling in Semiconductor Nanostructures. InHot Carriers in Semiconductor Nanostructures; Shah, J., Ed.; Academic Press: San Diego, 1992; pp 279−312.

(22) Trinh, M. T.; Houtepen, A. J.; Schins, J. M.; Hanrath, T.; Piris, J.; Knulst, W.; Goossens, A. P. L. M.; Siebbeles, L. D. A. In Spite of Recent Doubts Carrier Multiplication Does Occur in PbSe Nano-crystals.Nano Lett. 2008, 8, 1713−1718.

(23) Ellingson, R. J.; Beard, M. C.; Johnson, J. C.; Yu, P.; Micic, O. I.; Nozik, A. J.; Shabaev, A.; Efros, A. L. Highly Efficient Multiple Exciton Generation in Colloidal PbSe and Pbs Quantum Dots.Nano Lett. 2005, 5, 865−871.

(24) Moreels, I.; Lambert, K.; De Muynck, D.; Vanhaecke, F.; Poelman, D.; Martins, J. C.; Allan, G.; Hens, Z. Composition and Size-Dependent Extinction Coefficient of Colloidal PbSe Quantum Dots.Chem. Mater. 2007, 19, 6101−6106.

(25) Lloyd-Hughes, J.; Jeon, T.-I. A Review of the Terahertz Conductivity of Bulk and Nano-Materials. J. Infrared, Millimeter, Terahertz Waves 2012, 33, 871−925.

(26) Ambigapathy, R.; Bar-Joseph, I.; Oberli, D. Y.; Haacke, S.; Brasil, M. J.; Reinhardt, F.; Kapon, E.; Deveaud, B. Coulomb Correlation and Band Gap Renormalization at High Carrier Densities in Quantum Wires.Phys. Rev. Lett. 1997, 78, 3579−3582.

(27) Grozema, F. C.; Siebbeles, L. D. A. Mechanism of Charge Transport in Self-Organizing Organic Materials.Int. Rev. Phys. Chem. 2008,27, 87−138.

(28) Bhaskar, P.; Achtstein, A. W.; Diedenhofen, S. L.; Siebbeles, L. D. A. Mobility and Decay Dynamics of Charge Carriers in One-Dimensional Selenium Van Der Waals Solid.J. Phys. Chem. C 2017, 121, 18917−18921.

(29) Prins, P.; Grozema, F. C.; Schins, J. M.; Patil, S.; Scherf, U.; Siebbeles, L. D. A. High Intrachain Hole Mobility on Molecular Wires of Ladder-Type Poly(Para-Phenylenes). Phys. Rev. Lett. 2006, 96, 146601.

(30) Graham, R.; Yu, D. High Carrier Mobility in Single Ultrathin Colloidal Lead Selenide Nanowire Field Effect Transistors.Nano Lett. 2012,12, 4360−4365.

(31) Atkins, P. W.; Friedman, R. S.Molecular Quantum Mechanics; OUP Oxford, 2011.

(32) Barzykin, A. V.; Tachiya, M. Stochastic Models of Charge Carrier Dynamics in Semiconducting Nanosystems.J. Phys.: Condens. Matter 2007, 19, 065105.

The Journal of Physical Chemistry C pubs.acs.org/JPCC Article

https://dx.doi.org/10.1021/acs.jpcc.0c00541

J. Phys. Chem. C 2020, 124, 7550−7557 7557